PRL 96, 026804 (2006)

PHYSICAL REVIEW LETTERS week ending

20 JANUARY 2006

L**and**é g **Factors** **and** **Orbital** **Momentum** Quenching in Semiconductor Quantum Dots

Craig E. Pryor **and** Michael E. Flatté

Department **of** Physics **and** Astronomy **and** Optical Science **and** Technology Center, **University** **of** **Iowa**, **Iowa** City, **Iowa** 52242, USA

(Received 27 October 2004; published 18 January 2006)

We show that electron **and** hole L**and**é g factors in self-assembled III-V quantum dots have a rich

structure intermediate between that **of** paramagnetic atomic impurities **and** bulk semiconductors. Strain,

dot geometry, **and** confinement energy modify the effective g factors, yet are insufficient to explain our

results. We find that the dot’s discrete energy spectrum quenches the orbital angular momentum, pushing

the electron g factor towards 2, even when all the materials have negative bulk g factors. The approximate

shape **of** a dot can be determined from measurements **of** the g factor asymmetry.

DOI: 10.1103/PhysRevLett.96.026804 PACS numbers: 73.21.La, 76.30. v

An individual electron or hole spin in a single semiconductor

quantum dot provides an excellent system for testing

fundamental aspects **of** quantum dynamics **and** coherence.

The central quantity characterizing the response

**of** an electron or hole spin to an applied magnetic field, the

L**and**é g factor, has been measured optically [1–4] **and**

electrically [5–8]. For large dots [7–10], such as those

defined lithographically [7] or by electrical gates [8], the

magnetic fields **of** interest are usually large enough that the

magnetic length is smaller than the dot diameter. In this

limit the g factors are closely related to those **of** quantum

wells, **and** theory [9,11] appears to agree with experiment

[8]. The theoretical situation is much less satisfactory for

small dots—asymmetric structures grown by selfassembly

in the molecular beam epitaxy (MBE) growth

process or spherical nanocrystals grown by chemical synthesis.

Although several phenomena known to affect g

factors in quantum wells [12,13] have been explored in

quantum dots [14–20], the electronic states in dots are

discrete, **and** thus differ qualitatively from semiconductors

with unbounded motion in one or more directions [21].

Semiconductor quantum dots also have fully coherent

orbital electronic states with very long-lived spin coherence

[1], so the physics **of** their g factors is very different

from that **of** metallic nanoparticles [22–24] (whose g

factors are dominated by effects from incoherent orbital

scattering **and** spin scattering). The orbital coherence **of**

semiconductor quantum dot wave functions makes many

dot properties, such as the sharply peaked optical transitions,

resemble those **of** atoms more than bulk semiconductors.

If quantum dots are considered as ‘‘artificial

atoms’’ **and** approached with techniques developed for

magnetic atom dopants in solids [25], then the relevant

quantity is the ratio **of** the energy splitting between different

angular-momentum states to the spin-orbit interaction,

**and** for a strong confining potential the g factor **of** dots

should approach 2.

Here we show that the g factor **of** a ground-state electron

or hole in a quantum dot depends significantly on an

atomlike property: the quenching **of** orbital angular momentum

through quantum confinement. To identify this

effect we must consider also the known bulklike effects

on the g factors from dot strain **and** composition. These

include [14–19] the modification **of** the ground-state energy

in the dot, the relative proportion **of** dot or barrier

material the wave function occupies, **and** valence b**and**

mixing (typically **of** heavy **and** light states). In bulk semiconductors

the conduction-b**and** g factor is [26],

g 2

2E P

3E g E g

; (1)

where E g is the b**and** gap, is the spin-orbit coupling,

E P 2hSjPjXi 2 =m is the Kane energy involving S-like

**and** P-like Bloch functions hSj **and** hXj, respectively [12],

**and** m is the free electron mass. For unstrained spherical

InAs nanocrystals with hard wall boundary conditions only

E g changes, yet Eq. (1) is a very poor predictor **of** g factors

in these dots (Fig. 1).

The InAs in InAs=GaAs dots formed by self-assembly in

MBE is highly strained in order to accommodate the differing

lattice constants **of** InAs **and** the GaAs substrate. The

electron g factor predicted from Eq. (1) for InAs strained in

2E P ∆

g =2−

3E g(E g +∆)

FIG. 1 (color online). InAs nanocrystal electron g factor as a

function **of** dot size (parametrized by E g ). The effects **of** angularmomentum

quenching are clearly seen as g ! 2 for smaller

nanocrystals. 10 eV barriers were used to exclude the wave

function from the barriers. The dashed line shows the g factor

obtained from the bulk formula, using E g for the nanocrystal

(including the confinement energy).

0031-9007=06=96(2)=026804(4)$23.00 026804-1 © 2006 The American Physical Society

PRL 96, 026804 (2006)

PHYSICAL REVIEW LETTERS week ending

20 JANUARY 2006

⃗B in [001] direction

B⃗

in [110] direction

d [110]

e =

d[1¯10]

e =1.0

e =1.4

d [1¯10]

d [110]

e = d[110]

d [110]

e =1.0

e =1.4

B⃗

in [1¯10] direction

e = d [110]

d [110]

e =1.0

e =1.4

e = d[110] e =1.0

d [110] e =1.4

FIG. 2 (color online). InAs=GaAs quantum dot g factors for ~B

in the 001 direction as a function **of** the dot size (parametrized

by E g ) for various dot shapes. Solid lines are for the lowestenergy

electron; dashed lines are for the lowest energy hole.

Experimental values are from Ref. [5].

this way is negative, as is the known g factor for unstrained

GaAs. Yet the electron g factors for such dots are positive

over almost the entire size range (Fig. 2). Thus the bulklike

approach to g factors in these quantum dots, averaging the

g factors over the dot **and** barrier material [14,15], also

fails. The competing influence **of** atomlike **and** bulklike

effects predict that the growth-direction electron g factor

increases with increasing dot size, whereas considering

only bulklike effects leads to the opposite result. Our

results agree with recent experiments on electron g factors

[5]. We predict hole g factors have large positive values for

magnetic fields in the growth direction, **and** small negative

values in the in-plane directions (Figs. 2 **and** 3), **and** are

sensitive to dot shape. The calculations presented here are

for unstrained InAs spherical nanocrystals **and** strained

InAs=GaAs MBE-grown quantum dots, but our qualitative

conclusion—that the ‘‘artificial atom’’ viewpoint is vitally

important to underst**and**ing g factors—applies to all small

quantum dots.

Our results also point the way towards electric-field

control **of** g factors in quantum dots. g factor control via

manipulation **of** the electronic wave function in quantum

wells has already been used to control spin precession [27],

**and** to drive spin resonance [28]. Because **of** the large size

**of** quantum dots compared to atoms, moderate voltages

applied by electrical gates [21] can modify the dot shape,

energy levels, **and** g, **and** thus drive spin resonance in a

static magnetic field. Such control **of** electron spin resonance

in an individual quantum dot could assist ultrafast

manipulation **of** information encoded in electron or hole

026804-2

FIG. 3 (color online). InAs=GaAs quantum dot g factors along

the 110 **and** 110 directions as a function **of** dot size (parametrized

by E g ). Solid lines are for the lowest-energy electron;

dashed lines are for the lowest energy hole.

spin [29], as well as permit single-qubit gate operations for

quantum computation [30].

We calculated quantum dot g factors at T 0Kusing

8-b**and** strain dependent k p theory in the envelope approximation

with finite differences on a real space grid

[31]. g came from the spin splitting in a magnetic field **of**

jBj 0:1 T**and** the sign **of** g from the spin direction **of** the

lower energy state (parallel or antiparallel to ~B). Material

parameters were taken from Ref. [32].

The magnetic field was included by coupling to both the

envelope function **and** the spin. The envelope was coupled

to ~B using the st**and**ard prescription for introducing gauge

fields on a lattice. For example,

~r ^x ~r ^x

2

! ~r ^x U x ~r ~r ^x Ux y ~r ^x

2

; (2)

where is the grid spacing **and** U x ~r is the phase acquired

by an electron hopping from the site at ~r to the site at ~r

^x. The U’s were determined by the requirement that

transport around a plaquette produced the Aharonov-

Bohm phase corresponding to the encircled flux, for example

U x ~r U y ~r ^x Ux y ~r ^y Uy y ~r exp i 2 B ? e=@ ;

(3)

where B ? is the magnetic field component perpendicular to

the plaquette. The electron spin was coupled to ~B though a

Pauli term for the Bloch functions, given by

PRL 96, 026804 (2006)

H s

B

2 ~ B

0

1

2 ~ 0 0

B 4

@ 0 ~ 3

J 0

C

A; (4)

2

0 0

where B is the Bohr magneton **and** ~ **and** ~J are the spin

matrices for spin 1=2 **and** 3=2, respectively. The g factors

for the Bloch functions are 2, 4 3 , **and** 2 3

for the conduction,

valence, **and** spin-orbit b**and**s, respectively. The Bloch

function g factors are determined solely by the angular

momentum **of** the Bloch states.

As these numerical calculations are performed in a finite

box, numerical artifacts may arise if the total magnetic flux

through the box is not an integer number **of** the flux

quantum corresponding to a single electron [33]. To avoid

any such problems, the value **of** ~B was modified at the

edges **of** the box (within the barrier material) so as to make

the total flux in each **of** the x, y, **and** z directions an integer.

This allowed the use **of** both hard wall **and** periodic boundary

conditions, **and** comparison between the two boundary

conditions established that the box was sufficiently large to

avoid finite-size artifacts.

An advantage **of** this approach is that no further truncation

**of** the basis is done after a bulk b**and** basis is chosen.

Because the spin-orbit interaction is positive in the bulk

semiconductor constituents **of** the dot, it is energetically

favorable for the spin **and** orbital angular momenta to be

antiparallel to each other. (This is the ultimate reason for

the electron g2).

We now summarize the physical picture we have developed

to underst**and** the calculations shown in Figs. 1–3.

First consider the known origin **of** the effective g for

conduction electrons in a bulk semiconductor [26]. When

a magnetic field is applied, the orbital part **of** the wave

function is modified into L**and**au levels, corresponding to

quantized orbital angular momentum along the axis **of** the

magnetic field. In a single b**and** model the L**and**au levels’

orbital angular momentum comes from the envelope function

alone. When the conduction **and** valence b**and**s are

coupled, there is also a contribution from the valence Bloch

functions, which have a significant spin-orbit coupling.

The Zeeman energy now splits the lowest L**and**au level

into two spin-polarized L**and**au levels, one with spin parallel

to the quantized orbital angular momentum **and** one

antiparallel. Although the bare g 2 lowers the energy **of**

the parallel spin state **and** raises that **of** the antiparallel

state, the spin-orbit interaction preferentially aligns spin

antiparallel to the orbital angular momentum. When that

effect is absorbed into an effective g, it makes g

PRL 96, 026804 (2006)

PHYSICAL REVIEW LETTERS week ending

20 JANUARY 2006

is in the nanocrystal calculations **of** Fig. 1). Measurements

for large dots [5] are shown as well. These measurements

cannot determine the sign **of** the g factor; we identify the

sign to be positive based on our calculations.

Using Eq. (1) with E g **and** replaced by the values

calculated for bulk InAs with the same strain as the InAs in

the dot leads to the electron g 6. Increasing E g to

include the largest possible confinement energy for a dot

state gives g 0:5. The GaAs barrier has g 0:44,so

any averaging approach would produce a negative g factor,

**and** the g factor should decrease as the quantum dot size

increases. Because **of** orbital angular-momentum quenching

the actual electron g factors shown in Fig. 2 are

positive, except for the largest dots considered, which

have g 0:05, **and** the g factor increases as the quantum

dot size increases—the opposite trend.

As the approximate dot shape is frequently unknown, the

001 hole g factors (Fig. 2) or in-plane electron g factors

(Fig. 3) may be usable as diagnostics for the dot height, **and**

the in-plane hole g factors (Fig. 3) for the elongation. Use

**of** in-plane electron g factors to diagnose dot height may

be particularly effective because their dependence on E g

**and** e is weak. In-plane hole g factors, however, depend

strongly on both the height **and** elongation, but not on E g .

The in-plane hole g factors are much smaller in magnitude

than the hole g factors along the growth direction. This is

qualitatively similar to the results **of** Ref. [17] for Si=Ge

quantum dots. However, for InAs=GaAs quantum dots the

sign **of** the hole g factor differs for the growth direction **and**

in-plane. The large anisotropy for holes is due to the

valence state splitting caused by confinement **and** strain.

Whereas electron states with arbitrary spin direction can be

constructed from the spin-degenerate up **and** down states,

the hole states in a dot are not fourfold degenerate angularmomentum

3=2 states as in bulk materials, but are instead

split into two doublets (heavy **and** light holes) with differing

orbital angular momentum projected along the growthdirection

axis. This suppresses the formation **of** states with

arbitrary spin direction [13].

We have shown that the g factors in quantum dots are

dominated by the atomlike phenomenon **of** angularmomentum

quenching, leading to electron **and** hole g

factor values **and** trends that differ substantially from those

seen in bulk semiconductors, **and** are closer to the bare

value **of** 2. For InAs=GaAs dots, strain **and** geometric

asymmetry also contribute to g, **and** result in strong g

factor anisotropy, especially for hole states. Careful study

**of** the anisotropy **of** the hole g factors can provide approximate

information about the dot shape. Our unexpected

results for the electron **and** hole g factors suggest that the

‘‘artificial atom’’ picture promises additional surprises for

the physics **of** spin dynamics in quantum dots.

This work was supported by DARPA/ARO DAAD19-

01-1-0490.

[1] J. A. Gupta et al., Phys. Rev. B 59, R10421 (1999).

[2] M. Bayer et al., Phys. Rev. Lett. 82, 1748 (1999).

[3] A. R. Goñi et al., Jpn. J. Appl. Phys. 39, 3907 (2000).

[4] J. G. Tischler et al., Phys. Rev. B 66, 081310 (2002).

[5] G. Medeiros-Ribeiro, E. Ribeiro, **and** H. Westfahl, Jr.,

Appl. Phys. A 77, 725 (2003).

[6] G. Medeiros-Ribeiro et al., Appl. Phys. Lett. 80, 4229

(2002).

[7] L. P. Kouwenhoven, D. G. Austing, **and** S. Tarucha, Rep.

Prog. Phys. 64, 701 (2001).

[8] R. Hanson et al., Phys. Rev. Lett. 91, 196802 (2003).

[9] M. Valín-Rodríguez, A. Puente, **and** L. Serra, Phys. Rev. B

69, 085306 (2004).

[10] T. Darnh**of**er, D. A. Broido, **and** U. Rössler, Phys. Rev. B

50, 15 412 (1994).

[11] R. Kotlyar et al., Phys. Rev. B 63, 085310 (2001).

[12] E. L. Ivchenko **and** G. E. Pikus, Superlattices **and** Other

Heterostructures (Springer, New York, 1997).

[13] R. Winkler, Spin-Orbit Coupling Effects in Two-

Dimensional Electron **and** Hole Systems (Springer, New

York, 2003).

[14] A. A. Kiselev, E. L. Ivchenko, **and** U. Rössler, Phys. Rev.

B 58, 16 353 (1998).

[15] A. V. Rodina, Al. L. Efros, **and** A. Yu. Alekseev, Phys. Rev.

B 67, 155312 (2003).

[16] J. Schrier **and** K. B. Whaley, Phys. Rev. B 67, 235301

(2003).

[17] A. V. Nenashev, A. V. Dvurechenskii, **and** A. F. Zinovieva,

Phys. Rev. B 67, 205301 (2003).

[18] S. J. Prado et al., Phys. Rev. B 67, 165306 (2003).

[19] S. J. Prado et al., Physica (Amsterdam) 20E, 286 (2004).

[20] Y. P Krasny, N. P. Kovalenko, U. Krey, **and** L. Jacak,

J. Phys. Condens. Matter 13, 4341 (2001).

[21] D. Bimberg, M. Grundmann, **and** N. N. Ledentsov,

Quantum Dot Heterostructures (Wiley, New York, 1998).

[22] K. A. Matveev, L. I. Glazman, **and** A. I. Larkin, Phys. Rev.

Lett. 85, 2789 (2000).

[23] P. W. Brouwer, X. Waintal, **and** B. I. Halperin, Phys. Rev.

Lett. 85, 369 (2000).

[24] J. R. Petta **and** D. C. Ralph, Phys. Rev. Lett. 89, 156802

(2002).

[25] J. H. Van Vleck, The Theory **of** Electric **and** Magnetic

Susceptibilities (Oxford, New York, 1932).

[26] S. Zwerdling, B. Lax, L. M. Roth, **and** K. J. Button, Phys.

Rev. 114, 80 (1959); L. M. Roth, B. Lax, **and** S.

Zwerdling, Phys. Rev. 114, 90 (1959).

[27] G. Salis et al., Nature (London) 414, 619 (2001).

[28] Y. Kato et al., Science 299, 1201 (2003).

[29] Semiconductor Spintronics **and** Quantum Computation,

edited by D. Awschalom, D. Loss, **and** N. Samarth

(Springer-Verlag, Berlin, 2002).

[30] D. Loss **and** D. P. DiVincenzo, Phys. Rev. A 57, 120

(1998).

[31] C. Pryor, Phys. Rev. B 57, 7190 (1998).

[32] I. Vurgaftman, J. R. Meyer, **and** L. R. Ram-Mohan,

J. Appl. Phys. 89, 5815 (2001).

[33] C. Pryor, Phys. Rev. B 44, 12 473 (1991).

[34] C. E. Pryor **and** M. E. Flatté, Phys. Rev. Lett. 91, 257901

(2003).

026804-4